#------------------------------------------------------------------------------
#$Date: 2017-06-05 03:11:43 +0300 (Mon, 05 Jun 2017) $
#$Revision: 197405 $
#$URL: file:///home/coder/svn-repositories/cod/cif/4/34/57/4345749.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/
#
# All data on this site have been placed in the public domain by the
# contributors.
#
data_4345749
loop_
_publ_author_name
'Lü, Minfeng'
'Jo, Hongil'
'Oh, Seung-Jin'
'Lee, Suheon'
'Choi, Kwang-Yong'
'Yu, Yang'
'Ok, Kang Min'
_publ_section_title
;
 Syntheses, Structures, and Characterization of Quaternary Tellurites,
 Li3MTe4O11 (M = Al, Ga, and Fe).
;
_journal_issue                   10
_journal_name_full               'Inorganic chemistry'
_journal_page_first              5873
_journal_page_last               5879
_journal_paper_doi               10.1021/acs.inorgchem.7b00530
_journal_volume                  56
_journal_year                    2017
_chemical_formula_sum            'Ga2 Li6 O22 Te8'
_chemical_formula_weight         1553.88
_chemical_name_systematic        ' ?'
_space_group_IT_number           15
_symmetry_cell_setting           monoclinic
_symmetry_Int_Tables_number      15
_symmetry_space_group_name_Hall  '-C 2yc'
_symmetry_space_group_name_H-M   'C 1 2/c 1'
_cell_angle_alpha                90
_cell_angle_beta                 109.726(4)
_cell_angle_gamma                90
_cell_formula_units_Z            2
_cell_length_a                   18.7906(10)
_cell_length_b                   5.1841(2)
_cell_length_c                   10.7786(5)
_cell_measurement_reflns_used    5065
_cell_measurement_temperature    298.0
_cell_measurement_theta_max      28.405
_cell_measurement_theta_min      3.893
_cell_volume                     988.35(8)
_diffrn_ambient_temperature      298.0
_diffrn_measured_fraction_theta_full 0.98
_diffrn_measured_fraction_theta_max 0.97
_diffrn_measurement_device       CCD
_diffrn_measurement_device_type  'Bruker SMART BREEZE'
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_probe          x-ray
_diffrn_radiation_source         'X-ray tube'
_diffrn_radiation_type           'Mo K\a'
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0318
_diffrn_reflns_av_unetI/netI     0.0199
_diffrn_reflns_limit_h_max       25
_diffrn_reflns_limit_h_min       -25
_diffrn_reflns_limit_k_max       6
_diffrn_reflns_limit_k_min       -6
_diffrn_reflns_limit_l_max       14
_diffrn_reflns_limit_l_min       -14
_diffrn_reflns_number            8364
_diffrn_reflns_theta_full        28.61
_diffrn_reflns_theta_max         28.65
_diffrn_reflns_theta_min         2.3
_exptl_absorpt_coefficient_mu    14.41
_exptl_absorpt_correction_T_max  0.7457
_exptl_absorpt_correction_T_min  0.4350
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_process_details   Bruker
_exptl_crystal_colour            colorless
_exptl_crystal_density_diffrn    5.2213
_exptl_crystal_description       brick
_exptl_crystal_F_000             1344
_exptl_crystal_size_max          0.80
_exptl_crystal_size_mid          0.22
_exptl_crystal_size_min          0.20
_refine_diff_density_max         1.79
_refine_diff_density_min         -1.20
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_gt    1.87
_refine_ls_goodness_of_fit_ref   1.82
_refine_ls_number_constraints    0
_refine_ls_number_parameters     65
_refine_ls_number_reflns         1237
_refine_ls_number_restraints     0
_refine_ls_R_factor_all          0.0257
_refine_ls_R_factor_gt           0.0234
_refine_ls_shift/su_max          0.0234
_refine_ls_shift/su_mean         0.0024
_refine_ls_structure_factor_coef F
_refine_ls_weighting_details     w=1/(σ²(F)+0.0001F²)
_refine_ls_weighting_scheme      sigma
_refine_ls_wR_factor_gt          0.0305
_refine_ls_wR_factor_ref         0.0311
_reflns_number_gt                1139
_reflns_number_total             1237
_reflns_threshold_expression     I>3σ(I)
_cod_data_source_file            ic7b00530_si_002.cif
_cod_data_source_block           Li3GaTe4O11
_cod_depositor_comments
;
The following automatic conversions were performed:

'_diffrn_radiation_probe' value 'X-ray' changed to 'x-ray' according
to
/home/data/users/saulius/crontab/automatic-downloads/rss-feeds/ACS/lib/dictionaries/cif_core.dic
dictionary named 'cif_core.dic' version 2.4.2 from 2011-04-26.

Automatic conversion script
Id: cif_fix_values 4973 2017-02-22 13:04:09Z antanas 

 Adding full bibliography for 4345748--4345749.cif.
;
_cod_database_code               4345749
loop_
_space_group_symop_id
_space_group_symop_operation_xyz
1 x,y,z
2 -x,y,-z+1/2
3 -x,-y,-z
4 x,-y,z+1/2
5 x+1/2,y+1/2,z
6 -x+1/2,y+1/2,-z+1/2
7 -x+1/2,-y+1/2,-z
8 x+1/2,-y+1/2,z+1/2
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_adp_type
_atom_site_U_iso_or_equiv
_atom_site_site_symmetry_multiplicity
_atom_site_occupancy
_atom_site_calc_flag
Te1 Te 0.665366(19) 0.33437(6) 0.17008(3) Uani 0.01117(12) 8 1 d
Te2 Te 0.55606(2) 0.76199(6) -0.06245(4) Uani 0.01683(14) 8 1 d
Ga1 Ga 0.75 0.25 0.5 Uani 0.0093(3) 4 1 d
O1 O 0.6461(2) 0.8935(6) -0.0713(4) Uiso 0.0148(7) 8 1 d
O2 O 0.7241(2) 0.4320(6) 0.0694(3) Uiso 0.0116(6) 8 1 d
O3 O 0.7327(2) 0.4382(6) 0.3327(3) Uiso 0.0127(7) 8 1 d
O4 O 0.6103(2) 0.6448(7) 0.1520(4) Uiso 0.0194(8) 8 1 d
O5 O 0.5662(2) 0.4194(7) -0.0996(4) Uiso 0.0175(7) 8 1 d
O6 O 0.5 0.8761(11) -0.25 Uiso 0.0322(14) 4 1 d
Li1 Li 0.6721(7) 1.2531(17) -0.1149(11) Uani 0.024(4) 8 1 d
Li2 Li 0.5210(10) 0.263(3) -0.2704(19) Uani 0.017(6) 8 0.5 d
loop_
_atom_type_symbol
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
Ga 0.2307 1.6083 'International Tables Vol C tables 4.2.6.8 and 6.1.1.1'
Li -0.0003 0.0001 'International Tables Vol C tables 4.2.6.8 and 6.1.1.1'
O 0.0106 0.0060 'International Tables Vol C tables 4.2.6.8 and 6.1.1.1'
Te -0.5308 1.6751 'International Tables Vol C tables 4.2.6.8 and 6.1.1.1'
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle_site_symmetry_3
_geom_angle
O2 Te1 O3 . 96.98(16)
O2 Te1 O4 . 96.92(18)
O3 Te1 O4 . 91.45(15)
O1 Te2 O5 . 100.35(18)
O5 Li2 O5 2_654 120.6(9)
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_site_symmetry_2
_geom_bond_distance
Te1 O2 . 1.861(4)
Te1 O3 . 1.862(3)
Te1 O4 . 1.887(4)
Te2 O1 . 1.857(4)
Te2 O5 . 1.844(4)
Li1 O1 . 2.022(10)
Li2 O5 . 1.926(18)
Li2 O5 2_654 1.937(16)
